University of Bath M KOH at room temperature by cyclic voltammetry (CV, BioLogic, SP-50, USA) with a
Embed Size (px)
Transcript of University of Bath M KOH at room temperature by cyclic voltammetry (CV, BioLogic, SP-50, USA) with a
Citation for published version: Chandrasekaran, S, Kim, EJ, Chung, JS, Bowen, CR, Rajagopalan, B, Adamaki, V, Misra, RDK & Hur, SH 2016, 'High performance bifunctional electrocatalytic activity of a reduced graphene oxide-molybdenum oxide hybrid catalyst', Journal of Materials Chemistry A, vol. 4, no. 34, pp. 13271-13279. https://doi.org/10.1039/c6ta05043c
Publication date: 2016
Document Version Peer reviewed version
Link to publication
The final publication is available at the Royal Society of Chemistry via 10.1039/c6ta05043c
University of Bath
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Take down policy If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Download date: 31. Oct. 2020
https://doi.org/10.1039/c6ta05043c https://doi.org/10.1039/c6ta05043c https://researchportal.bath.ac.uk/en/publications/high-performance-bifunctional-electrocatalytic-activity-of-a-reduced-graphene-oxidemolybdenum-oxide-hybrid-catalyst(557fc8bf-eb06-4eaa-bcab-e4a986b9b2f7).html
Please do not adjust margins
Received 00th January 20xx, Accepted 00th January 20xx
High performance bifunctional electrocatalytic activity of a reduced graphene oxide - molybdenum oxide hybrid catalyst Sundaram Chandrasekarana, Eui Jung Kima, Jin Suk Chunga, Chris R Bowenb, Balasubramaniyan Rajagopalana, Vaia Adamaki b, R.D.K. Misrac, and Seung Hyun Hur*a
The advances in cost effective, highly active and stable electrocatalysts for the oxygen reduction reaction (ORR) and the oxygen evolution reaction (OER) remain the major issues for the commercialization of metal air-batteries and alkaline fuel cells. In this aspect, a facile hydrothermal route was developed to prepare nonprecious metal electrocatalysts including pristine MoO3 rods, nanospheres, and their hybrids with reduced graphene oxide (rGO). This is the first report of the use of rGO coupled with hexagonal MoO3 nanocrystals to act as both ORR and OER catalysts. The rGO - MoO3 sphere hybrid catalyst exhibited excellent catalytic activity toward both the ORR and OER than pristine MoO3 rods, MoO3 spheres and rGO- MoO3 rods. In addition, the rGO - MoO3 nanosphere hybrid exhibited excellent catalytic activity, long-term durability, and CO tolerance compared to a high quality commercial Pt/C catalyst. This makes the GMS hybrid composite a highly promising candidate for high-performance non-precious metal-based bi-functional electrocatalysts with low cost and high efficiency for electrochemical energy conversion. The enhanced activity of the rGO - MoO3 nanosphere hybrid is due mainly to the enhanced structural openness in the tunnel structure of the hexagonal MoO3 when it is coupled with rGO.
1. Introduction The advancement of cost effective, naturally abundant,
environmentally benign, and highly active catalysts for energy conversion and storage is of utmost importance and is an important topic in renewable energy research1-4. In particular, water splitting5, fuel cells6 and metal-air batteries7 are required for future energy conversion and storage applications as a result of their high theoretical energy density. The oxygen reduction reaction (ORR) and oxygen evolution reaction (OER) play major roles in these devices. In this context, the discovery of robust materials for both the OER and ORR is important but also very challenging. Traditional catalysts, such as Pt and its alloys, perform well for the ORR, but their high cost limits their applications8-11. Materials such as, iridium and ruthenium- based compounds and their oxides are well known OER catalysts12-14. These metals are also expensive and among the rarest elements on earth, making them impractical for large- scale applications. Therefore, alternative catalysts based on cost effective, metal-free materials or non-precious metals have attracted considerable attention4. As a result, a number of non-precious nanomaterials, such as Ni0.2Co0.3Ce0.5Ox
16 and Ni3S2 17, have been explored for their high OER
activity. Recently, a range of uni-functional carbon materials or metal oxides with carbon materials also have been reported to
exhibit high activities either for the OER or for ORR activity18-23. However, the use of single catalyst as a bi-functional catalyst24- 32 has rarely been reported because the bi-functionality requires significantly low over potentials and high activities for both the OER and ORR. Therefore, it remains a considerable challenge to design a high-performance catalyst capable of unifying the both OER and ORR for energy conversion and storage applications with the relevant properties of high activity, low-cost, carbon monoxide (CO) tolerance, and excellent stability.
Recently, a wide range of molybdenum oxide-based compounds with the manifold structural motifs and properties have attracted considerable interest in the field of materials research. These materials have been shown to exhibit excellent properties for catalysis33, 34, photocatalysis35, batteries36, solar energy conversion37, 38, and sensors39, 40. In crystallographic view, MoO3 exists in three phases, orthorhombic α-MoO3, monoclinic β-MoO3, and hexagonal H- MoO3. The hexagonal H-MoO3 system is a metastable phase, which is constructed from the zigzag chains of octahedral [MoO6] as the building blocks attached through adjacent oxygen. Compared to α and β crystal structures, hexagonal MoO3 retains a number of interesting properties. The tunnel structure of H-MoO3 can result in electron-hole separation and afford large special locations for cation insertion and extraction41. To date, there are no reports of multifunctional catalysts based on a hexagonal molybdenum oxide embedded graphene material for ORR and OER activity. Importantly the three essential factors to achieve in commercializing fuel technologies include high efficiency, stability, and scalability42. In this regard, the present study focused on a catalyst that is not only highly active but is also facile, robust, highly stable, and easily scalable. This paper reports the first, highly active
ARTICLE Journal Name
Please do not adjust margins
Please do not adjust margins
and multifunctional reduced graphene oxide (rGO) - hexagonal MoO3 hybrid catalysts synthesized via a facile hydrothermal route. For sample identification, the prepared MoO3 rods, MoO3 nanospheres, rGO-MoO3 rods, and rGO-MoO3 nanosphere samples are denoted as MR, MS, GMR, and GMS respectively. The synthesized materials were tested for both the ORR and OER reactions and GMS hybrid shows promising performance compared to a high quality commercial Pt/C catalyst, indicating its potential as a cost effective and highly active bi-functional catalyst.
2.1 Catalysts Synthesis In a typical procedure of MR, 3 mmol of ammonium heptamolybdate tetrahydrate ((NH4)6Mo7O2.4H2O) was dissolved in 50 mL of distilled water and 3 mmol HCl was then added to the reaction solution with vigorous stirring. The resulting solution was transferred to a 100 mL Teflon-lined stainless autoclave and sealed tightly, which was kept at 180 °C for 14 h. The autoclave was then allowed to cool naturally to room temperature. The resulting products were filtered, washed several times with absolute ethanol and distilled water, and dried at 250 °C for 4 h. The MS sample was synthesized using the same procedure, only the HCl was replaced with ammonia.
The graphene oxide (GO) was synthesized from graphite powders using a modified Hummers’ method. In a typical synthesis of the GMR or GMS, 20 mg of MR or MS was added gradually to 20 mL of the GO solution. The mixture solution was then stirred magnetically, and 5 mL of ammonia was added gradually to the mixture. After 2 h, the resulting stable suspension was then transferred to a Teflon-lined autoclave, and treated hydrothermally at 180 °C for 14 h. Finally, the as- prepared product was dried at 250 °C for 4 h. 2.2 Instrumental analysis
The crystalline phases were identified by X-ray diffraction (XRD; Rigaku) using Cu-Kα radiation. The surface morphologies were identified by field emission scanning electron microscopy (FE-SEM; JSM 6500F) and transmission electron microscopy (TEM; JEOL JEM 2100F). The vibrational, rotational and other low-frequency modes in the sample were analyzed by Raman spectroscopy (Thermo Scientific DXR). The material composition and oxidation states of carbon and iron atoms in the GMS nanocomposites were analyzed by X-ray photoelectron spectroscopy (XPS, Thermo Scientific K-alpha). N2 adsorption–desorption measurements were carried out at 77 K using a Micromeritics ASAP 2020 gas-sorption system. Thermogravimetric analysis (TGA) was